Microstructure and Mechanical Properties of Copper Billets ... Microstructure and Mechanical...
Embed Size (px)
Transcript of Microstructure and Mechanical Properties of Copper Billets ... Microstructure and Mechanical...
Microstructure and Mechanical Properties of CopperBillets Fabricated by the Repetitive Extrusion and Free
Forging ProcessYang Wu, Shuhai Huang, Qiang Chen, Bo Feng, Dayu Shu, and Zhiwei Huang
(Submitted August 10, 2018; in revised form January 10, 2019; published online February 14, 2019)
In the present study, with the aim of obtaining a weakened texture, grain refinement and improvedmechanical properties, copper billets were successfully fabricated using the severe plastic deformationmethod of repetitive extrusion and free forging (REFF) without using any additional tools or devices. Theevolution of the microstructure, texture and mechanical behavior of the ultrafine grain copper billets overan increasing number of REEF cycles was also systematically studied. Our results show that the effectivestrain per REFF process was e = 2.35. After two cycles of REFF process, the sum effective strain becamee = 4.7, leading to high efficiency of grain refinement. The grain size was refined from 50 to 0.8 lm; theyield strength was increased to 462 MPa, and we obtained a weakened texture in the pure copper billets. Byincreasing the number of cycles, the grain refinement ability was decreased, and the texture was thusstrengthened further. Therefore, two cycles of REFF were a reasonable process for producing ultrafine-grained copper billets.
Keywords microstructure, pure copper, repetitive extrusion andfree forging, texture
Pure copper and its alloys with the high electrical andthermal conductivity, high formability, machinability andrelatively moderate properties are increasingly being concernedin many industries (Ref 1-3). However, pure copper ingots,prepared by casting, are composed primarily of coarse-grained(CG) microstructures (Ref 4). For some applications, thesemicrostructures are not a problem because these applications donot depend on isotropic or superior mechanical properties, butfor particular applications, it is important for the Cu to haveultrafine-grained (UFG) microstructures and extremely uniformmechanical properties. For instance, some of these applicationsinclude use as thin sheets for co-deformation with pure Cu forNb3Sn superconductor diffusion barriers or as thick sheet disksfor explosively formed penetrators (Ref 5). Without uniformityof microstructure, a weakened texture and a grain refinementmicrostructure, the characteristics of uniform deformation areabsent and problems such as orange peel surface roughness,non-uniform thinning and premature facture can arise (Ref 6-8).
Ultrafine-grained materials have spawned much interest infields where extremely high tensile and yield strength arenecessary for construction, as an alternative to coarse-grained
(CG) counterparts for satisfactory ductility (Ref 4, 9). Acommonly used set of methods for fabricating UFG materials isthe severe plastic deformation (SPD) methods, of which thebest-known SPD techniques for producing UFG materials arethe equal-channel angular pressing (ECAP) and the high-pressure torsion (HPT) (Ref 10-14). Various UFG SPDmaterials (e.g., Cu (Ref 15, 16), Al (Ref 17), Ta (Ref 18), Ti(Ref 19) and steel (Ref 6)) have been prepared using ECAP orHPT processing. Microstructures can be refined to equiaxedsubgrains, which is accompanied by a significant increase witha satisfactory ductility. However, materials produced by ECAPand HPT have a small size along the transverse direction (Ref20). This can limit the industrial applications of these methodsfor producing bulk billets for post-forging.
Extrusion and forging processes are suitable for preparingUFG materials at room or slightly above. It is well known thatextrusion and free forging processes are highly efficient andsimple, making them ideal for industrial applications. There-fore, we propose to combine these two traditional processes incyclic processes of conventional direct extrusion and by freeforging, a process termed repetitive extrusion and free forging(REFF). Compared with other SPD methods, REFF has severaladvantages, such as a higher strain per cycle, more shear planesand a more effective grain fragmentation. A similar approach,repetitive extrusion and upsetting (REU), has been reported bysome publications (Ref 21). One publication reported theapplication of the REU process for fabricating pure aluminumbillets with only 20 mm length along the longitudinal directionand 30 mm along the transverse direction. Unfortunately, thissize of REU billets was insufficient to meet the needs ofindustrial applications. However, compared with REU, REFFhas several advantages of a higher strain per cycle, a lowerworking force and no need for any additional tools or devices.Thus, REFF processing should be suitable for efficient andcost-saving industrial applications. In the present study, bulksize pure copper billets with excellent grain refinementmicrostructure for industry application, 80 mm in length along
Yang Wu, Shuhai Huang, Qiang Chen, Dayu Shu, andZhiwei Huang, Southwest Technology and Engineering ResearchInstitute, Chongqing 400039, China; and Bo Feng, GuangdongInstitute of Materials and Processing, Guangdong Academy ofSciences, Guangzhou 510650, China. Contact e-mail:email@example.com.
JMEPEG (2019) 28:20632070 The Author(s)https://doi.org/10.1007/s11665-019-03898-3 1059-9495/$19.00
Journal of Materials Engineering and Performance Volume 28(4) April 20192063http://crossmark.crossref.org/dialog/?doi=10.1007/s11665-019-03898-3&domain=pdfhttp://crossmark.crossref.org/dialog/?doi=10.1007/s11665-019-03898-3&domain=pdf
the longitudinal direction and 90 mm along the transversedirection, were successfully fabricated from coarse-grainedpure Cu. Three cyclic REFF passes were achieved in this work.The microstructure, texture evolution and mechanical proper-ties of the extrusion and forging of pure Cu from each REFFcycle pass were also systematically studied.
2. Experiments and Methods
2.1 REFF Process and Mechanical Tests
Commercially pure copper ingots containing coarse-grained(CG) counterparts and fully annealed condition were used forthe fabrication of the UFG copper billets. As shown in Fig. 1,the CG pure copper was machined into a cylinder with 90 mmin diameter and 80 mm in length. This ingot was kept in afurnace at 660 C for 2 h and then cooled at room temperaturein order to obtain a complete recrystallized microstructure.Before testing, the billets were covered with lubricant zincstearate and then were extruded at room temperature using anextrusion rate of 10 mm/s. The final extruded bar had adiameter of 50 mm. After complete extrusion, the extruded barwas free forged at the same rate until the initial diameter(90 mm) was reached again, so that the extrusion process couldbe repeated. For tensile tests, the dog-bone-shaped specimenswith a gauge length of 35 mm and a diameter of 5 mm were cutalong the longitudinal direction (ED or FD). Here, ED and FDrefer to the extrusion direction and free forging direction,respectively. Tensile tests were performed on a Shimadzumechanical testing system, using a strain rate of 103/s at roomtemperature. Each mechanical test was repeated three times.
2.2 Characterization of Microstructure and Texture
For studying the structural evolution, samples were cut fromthe center of the specimen perpendicular to the compressionplane and parallel to the ED and/or FD. The obtained surfacewas polished and subsequently etched. Electron backscattereddiffraction (EBSD) analyses were conducted on a FEI Nova400 SEM equipped with an HKL Chanel 5 system, using a stepsize of 1 lm for the initial CG Cu material and the firstextrusion billets, 0.3 lm for the first forging billet and thesecond extrusion billets and 0.15 lm for the second forgingbillets. Each specimen was scanned at three different areas tomeasure the average grain size. The samples for EBSDmapping were mechanically ground, followed by electrochem-ical polishing for 7 s at 273 K in the electrolyte solution of50% H3PO4, 25% distilled water and 25% alcohol at a DCvoltage of 6.5 V. The EBSD data were analyzed using theChannel 5 software. Grain boundaries were identified using 2minimum disorientation angle between two adjacent pixels,which led to the identification of grains having continuousclosed boundaries with at least a 2 grain boundary angle. Grainorientations were then defined as the average of the pixelorientations constituting the grain, and then misorientationangle between adjacent grains was obtained using these averagevalues (Ref 22).
3. Results and Discussion
3.1 Repetitive Extrusion and Free Forging Process
The present study shows that ultrafine-grained copper billetwith bulk size for industry applications could be successfully
Fig. 1 Schematic diagrams of the cyclic REFF process
2064Volume 28(4) April 2019 Journal of Materials Engineering and Performance
fabricated from CG Cu ingots using the REFF process. Duringeach cycle of the REFF process, a high effective strain and anaverage von Mises strain from the geometric dimensions of thedie using the normal components of the strain tensor wereobtained, as defined below (Ref 21):
e 4 lnDd
For the extrusion process, the diameter of the initial CGcopper ingot and the extruded UFG copper was replaced by D(90 mm) and d (50 mm), as shown in Fig. 1, respectively.Therefore, the extrusion ratio was 3.24, and the correspondingeffective strain per REFF process was e = 2.35. After twocycles, the sum effective strain became e = 4.7. Because thestrain value in the center position was very close to the strainvalue of calculation, and it generally increases from the centerto the surface of the Cu billet, so the microstructure of the billetsurface was preferentially refined (Ref 22). In order to obtainwhether a homogeneous microstructure from the center to